**Chemical:** Dibromoethyl Benzene

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibromoethyl Benzene | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibromoethyl Benzene — Chemical resistance ratings for common elastomers


**Chemical:** Dibutyl Cellosolve Adipate

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutyl Cellosolve Adipate | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutyl Cellosolve Adipate — Chemical resistance ratings for common elastomers


**Chemical:** Dibutyl Ether

**Nitrile (NBR):** 4

**EPDM:** 3

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 3

**Polyacrylate (ACM):** 3

**Hypalon (CSM):** 4

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 3

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutyl Ether | 4 | 3 | 4 | 4 | 4 | 3 | 3 | 4 | 3 | 2 | 3 | 3 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutyl Ether — Chemical resistance ratings for common elastomers


**Chemical:** Dibutyl Methylenedithio Glycolate

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutyl Methylenedithio Glycolate | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutyl Methylenedithio Glycolate — Chemical resistance ratings for common elastomers


**Chemical:** Dibutyl Phthalate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 3

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 3

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutyl Phthalate | 4 | 2 | 4 | 4 | 2 | 3 | 4 | 4 | 3 | 3 | 3 | 3 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutyl Phthalate — Chemical resistance ratings for common elastomers


**Chemical:** Dibutyl Sebacate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 2

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutyl Sebacate | 4 | 2 | 4 | 4 | 2 | 2 | 4 | 4 | 2 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutyl Sebacate — Chemical resistance ratings for common elastomers


**Chemical:** Dibutyl Thioglycolate

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutyl Thioglycolate | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutyl Thioglycolate — Chemical resistance ratings for common elastomers


**Chemical:** Dibutyl Thiourea

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutyl Thiourea | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutyl Thiourea — Chemical resistance ratings for common elastomers


**Chemical:** Dibutylamine

**Nitrile (NBR):** 4

**EPDM:** 1

**Neoprene (CR):** 3

**SBR:** 4

**Silicone (VMQ):** 3

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 4

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dibutylamine | 4 | 1 | 3 | 4 | 3 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dibutylamine — Chemical resistance ratings for common elastomers


**Chemical:** Dichloroacetic Acid

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloroacetic Acid | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloroacetic Acid — Chemical resistance ratings for common elastomers


**Chemical:** Dichloroaniline

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloroaniline | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloroaniline — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorobenzene or o-Dichlorobenzene

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 4

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorobenzene or o-Dichlorobenzene | 4 | 4 | 4 | 4 | X | 4 | 4 | 2 | 1 | 4 | 4 | 4 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorobenzene or o-Dichlorobenzene — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorobenzene or p-Dichlorobenzene

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 4

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorobenzene or p-Dichlorobenzene | 4 | 4 | 4 | 4 | X | 4 | 4 | 2 | 1 | 4 | 4 | 4 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorobenzene or p-Dichlorobenzene — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorobutane

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorobutane | 2 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorobutane — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorobutene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorobutene | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorobutene — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorodiphenyl-Dichloroethane (DDD)

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorodiphenyl-Dichloroethane (DDD) | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorodiphenyl-Dichloroethane (DDD) — Chemical resistance ratings for common elastomers


**Chemical:** Dichloroethane

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloroethane | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloroethane — Chemical resistance ratings for common elastomers


**Chemical:** Dichloroethylene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloroethylene | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloroethylene — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorohydrin

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorohydrin | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorohydrin — Chemical resistance ratings for common elastomers


**Chemical:** Dichloroisopropyl Ether

**Nitrile (NBR):** 4

**EPDM:** 3

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 3

**Hypalon (CSM):** 4

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 3

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloroisopropyl Ether | 4 | 3 | 4 | 4 | 4 | 4 | 3 | 4 | 3 | 2 | 3 | 3 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloroisopropyl Ether — Chemical resistance ratings for common elastomers


**Chemical:** Dichloromethane

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloromethane | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloromethane — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorophenol

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorophenol | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorophenol — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorophenoxyacetic Acid

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorophenoxyacetic Acid | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorophenoxyacetic Acid — Chemical resistance ratings for common elastomers


**Chemical:** Dichloropropane

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloropropane | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloropropane — Chemical resistance ratings for common elastomers


**Chemical:** Dichloropropene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichloropropene | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichloropropene — Chemical resistance ratings for common elastomers


**Chemical:** Dichlorosilane

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dichlorosilane | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dichlorosilane — Chemical resistance ratings for common elastomers


**Chemical:** Dicyclohexylamine

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 4

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dicyclohexylamine | 1 | 4 | 4 | 4 | 2 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dicyclohexylamine — Chemical resistance ratings for common elastomers


**Chemical:** Dicyclohexylammonium Nitrate

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dicyclohexylammonium Nitrate | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dicyclohexylammonium Nitrate — Chemical resistance ratings for common elastomers


**Chemical:** Dieldrin

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dieldrin | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dieldrin — Chemical resistance ratings for common elastomers


**Chemical:** Diesel Oil

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 3

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 3

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diesel Oil | 1 | 4 | 3 | 4 | 4 | 4 | 1 | 3 | 1 | 3 | 1 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diesel Oil — Chemical resistance ratings for common elastomers


**Chemical:** Diethanolamine (DEA)

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethanolamine (DEA) | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethanolamine (DEA) — Chemical resistance ratings for common elastomers


**Chemical:** Diethyl Benzene

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 1

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethyl Benzene | X | X | X | X | X | X | X | X | 1 | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethyl Benzene — Chemical resistance ratings for common elastomers


**Chemical:** Diethyl Carbonate

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethyl Carbonate | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethyl Carbonate — Chemical resistance ratings for common elastomers


**Chemical:** Diethyl Ether

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 3

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 3

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 4

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethyl Ether | 4 | 4 | 3 | 4 | 4 | 4 | 3 | 4 | 4 | 1 | 3 | 4 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethyl Ether — Chemical resistance ratings for common elastomers


**Chemical:** Diethyl Phthalate

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethyl Phthalate | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethyl Phthalate — Chemical resistance ratings for common elastomers


**Chemical:** Diethyl Sebacate

**Nitrile (NBR):** 2

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 2

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethyl Sebacate | 2 | 2 | 4 | 4 | 2 | 2 | 4 | 4 | 2 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethyl Sebacate — Chemical resistance ratings for common elastomers


**Chemical:** Diethyl Sulfate

**Nitrile (NBR):** 4

**EPDM:** 1

**Neoprene (CR):** 4

**SBR:** X

**Silicone (VMQ):** 2

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 3

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethyl Sulfate | 4 | 1 | 4 | X | 2 | X | X | X | 3 | X | X | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethyl Sulfate — Chemical resistance ratings for common elastomers


**Chemical:** Diethylamine

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethylamine | 2 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 4 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethylamine — Chemical resistance ratings for common elastomers


**Chemical:** Diethylaniline

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethylaniline | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethylaniline — Chemical resistance ratings for common elastomers


**Chemical:** Diethylene Glycol

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 2

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethylene Glycol | 1 | 1 | 1 | 1 | 2 | 1 | 2 | 1 | 1 | 4 | 1 | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethylene Glycol — Chemical resistance ratings for common elastomers


**Chemical:** Diethylenetriamine

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diethylenetriamine | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diethylenetriamine — Chemical resistance ratings for common elastomers


**Chemical:** Difluorodibromomethane

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** X

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Difluorodibromomethane | 4 | 2 | 4 | 4 | 4 | 2 | 4 | 4 | X | 4 | X | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Difluorodibromomethane — Chemical resistance ratings for common elastomers


**Chemical:** Difluoroethane

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Difluoroethane | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Difluoroethane — Chemical resistance ratings for common elastomers


**Chemical:** Difluoromonochloroethane

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Difluoromonochloroethane | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Difluoromonochloroethane — Chemical resistance ratings for common elastomers


**Chemical:** Diglycol Chloroformate

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diglycol Chloroformate | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diglycol Chloroformate — Chemical resistance ratings for common elastomers


**Chemical:** Diglycolic Acid

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diglycolic Acid | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diglycolic Acid — Chemical resistance ratings for common elastomers


**Chemical:** Dihydroxydiphenylsulfone

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dihydroxydiphenylsulfone | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dihydroxydiphenylsulfone — Chemical resistance ratings for common elastomers


**Chemical:** Diisobutyl Ketone

**Nitrile (NBR):** X

**EPDM:** 1

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** 1

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisobutyl Ketone | X | 1 | X | X | X | 1 | X | X | X | X | X | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisobutyl Ketone — Chemical resistance ratings for common elastomers


**Chemical:** Diisobutylcarbinol

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisobutylcarbinol | 1 | 4 | 2 | 4 | 2 | 4 | 1 | 2 | 1 | 1 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisobutylcarbinol — Chemical resistance ratings for common elastomers


**Chemical:** Diisobutylene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisobutylene | 2 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 3 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisobutylene — Chemical resistance ratings for common elastomers


**Chemical:** Diisooctyl Sebacate

**Nitrile (NBR):** 3

**EPDM:** 3

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 3

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 2

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisooctyl Sebacate | 3 | 3 | 4 | 4 | 3 | 4 | 4 | 4 | 2 | 4 | 3 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisooctyl Sebacate — Chemical resistance ratings for common elastomers


**Chemical:** Diisopropyl Ether (DIPE)

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisopropyl Ether (DIPE) | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisopropyl Ether (DIPE) — Chemical resistance ratings for common elastomers


**Chemical:** Diisopropyl Ketone

**Nitrile (NBR):** 4

**EPDM:** 1

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisopropyl Ketone | 4 | 1 | 4 | 4 | 4 | 1 | 4 | 4 | 4 | 4 | 4 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisopropyl Ketone — Chemical resistance ratings for common elastomers


**Chemical:** Diisopropylbenzene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisopropylbenzene | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisopropylbenzene — Chemical resistance ratings for common elastomers


**Chemical:** Diisopropylidene Acetone

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diisopropylidene Acetone | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diisopropylidene Acetone — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Acetamide

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Acetamide | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Acetamide — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Ether

**Nitrile (NBR):** 1

**EPDM:** 2

**Neoprene (CR):** 3

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 2

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 4

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Ether | 1 | 2 | 3 | X | X | X | X | X | 2 | X | X | 4 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Ether — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Formaldehyde

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Formaldehyde | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Formaldehyde — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Formamide (DMF)

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 3

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Formamide (DMF) | 2 | 1 | 3 | 4 | 2 | 2 | 4 | 4 | 4 | 4 | 4 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Formamide (DMF) — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Phenyl Carbinol

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Phenyl Carbinol | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Phenyl Carbinol — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Phenyl Methanol

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Phenyl Methanol | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Phenyl Methanol — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Phthalate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 2

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Phthalate | 4 | 2 | 4 | 4 | X | 2 | 4 | 4 | 2 | X | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Phthalate — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Sulfoxide (DMSO)

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Sulfoxide (DMSO) | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Sulfoxide (DMSO) — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyl Terephthalate (DMT)

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyl Terephthalate (DMT) | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyl Terephthalate (DMT) — Chemical resistance ratings for common elastomers


**Chemical:** Dimethylamine (DMA)

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 2

**SBR:** 2

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 3

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethylamine (DMA) | 2 | 1 | 2 | 2 | 2 | 2 | 4 | 3 | 4 | 3 | 4 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethylamine (DMA) — Chemical resistance ratings for common elastomers


**Chemical:** Dimethylaniline (Xylidine)

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethylaniline (Xylidine) | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethylaniline (Xylidine) — Chemical resistance ratings for common elastomers


**Chemical:** Dimethyldisulfide (DMDS)

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethyldisulfide (DMDS) | 1 | 4 | 2 | 4 | 2 | 4 | 1 | 2 | 1 | 1 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethyldisulfide (DMDS) — Chemical resistance ratings for common elastomers


**Chemical:** Dimethylhydrazine

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dimethylhydrazine | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dimethylhydrazine — Chemical resistance ratings for common elastomers


**Chemical:** Dinitrochlorobenzene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dinitrochlorobenzene | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dinitrochlorobenzene — Chemical resistance ratings for common elastomers


**Chemical:** Dinitrogen Tetroxide

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 2

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dinitrogen Tetroxide | X | X | X | X | X | X | X | X | X | X | X | X | 2 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dinitrogen Tetroxide — Chemical resistance ratings for common elastomers


**Chemical:** Dinitrotoluene (DNT)

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 4

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dinitrotoluene (DNT) | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dinitrotoluene (DNT) — Chemical resistance ratings for common elastomers


**Chemical:** Dioctyl Phthalate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 3

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 2

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dioctyl Phthalate | 4 | 2 | 4 | 4 | 3 | 2 | 4 | 4 | 2 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dioctyl Phthalate — Chemical resistance ratings for common elastomers


**Chemical:** Dioctyl Sebacate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 3

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 2

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dioctyl Sebacate | 4 | 2 | 4 | 4 | 3 | 2 | 4 | 4 | 2 | 2 | 3 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dioctyl Sebacate — Chemical resistance ratings for common elastomers


**Chemical:** Dioctylamine

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dioctylamine | 1 | 4 | 2 | 4 | 2 | 4 | 1 | 2 | 1 | 1 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dioctylamine — Chemical resistance ratings for common elastomers


**Chemical:** Dioxane

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 3

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dioxane | 4 | 2 | 4 | 4 | 4 | 2 | 4 | 4 | 4 | 4 | 4 | 3 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dioxane — Chemical resistance ratings for common elastomers


**Chemical:** Dioxolane

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 3

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 3

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dioxolane | 4 | 2 | 4 | 4 | 4 | 3 | 4 | 4 | 4 | 4 | 4 | 3 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dioxolane — Chemical resistance ratings for common elastomers


**Chemical:** Dipentene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dipentene | 2 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dipentene — Chemical resistance ratings for common elastomers


**Chemical:** Diphenyl Oxides

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 3

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diphenyl Oxides | 4 | 4 | 4 | 4 | 3 | 4 | 4 | 4 | 1 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diphenyl Oxides — Chemical resistance ratings for common elastomers


**Chemical:** Diphenyl

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diphenyl | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diphenyl — Chemical resistance ratings for common elastomers


**Chemical:** Diphenylamine (DPA)

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diphenylamine (DPA) | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diphenylamine (DPA) — Chemical resistance ratings for common elastomers


**Chemical:** Diphenylene Oxide

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diphenylene Oxide | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diphenylene Oxide — Chemical resistance ratings for common elastomers


**Chemical:** Diphenylpropane

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Diphenylpropane | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Diphenylpropane — Chemical resistance ratings for common elastomers


**Chemical:** Disilane

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Disilane | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Disilane — Chemical resistance ratings for common elastomers


**Chemical:** Dodecylbenzene

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dodecylbenzene | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dodecylbenzene — Chemical resistance ratings for common elastomers


**Chemical:** Dow Chemical 50-4

**Nitrile (NBR):** X

**EPDM:** 1

**Neoprene (CR):** 2

**SBR:** 1

**Silicone (VMQ):** X

**Butyl (IIR):** 2

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 2

**Viton (FKM):** 4

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 2

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Chemical 50-4 | X | 1 | 2 | 1 | X | 2 | X | 2 | 4 | X | 4 | 2 | 2 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Chemical 50-4 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Chemical ET378

**Nitrile (NBR):** 4

**EPDM:** X

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 3

**Hypalon (CSM):** 4

**Viton (FKM):** X

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** X

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Chemical ET378 | 4 | X | 4 | 4 | 4 | 4 | 3 | 4 | X | 2 | X | X | X |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Chemical ET378 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Chemical ET588

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 2

**SBR:** 1

**Silicone (VMQ):** X

**Butyl (IIR):** 2

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 2

**Viton (FKM):** 4

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 2

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Chemical ET588 | 3 | 1 | 2 | 1 | X | 2 | X | 2 | 4 | X | 4 | 2 | 2 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Chemical ET588 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -11

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -11 | 2 | 1 | 1 | 1 | 2 | 1 | 1 | 1 | 1 | 1 | 1 | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -11 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning 1208, 4050, 6620, F-60, XF-60

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 1

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning 1208, 4050, 6620, F-60, XF-60 | 1 | 1 | 1 | X | X | X | X | X | 1 | X | X | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning 1208, 4050, 6620, F-60, XF-60 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -1265 Fluorosilicone Fluid

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 1

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -1265 Fluorosilicone Fluid | 2 | 1 | 1 | 1 | 1 | 1 | 1 | 1 | 1 | 1 | 3 | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -1265 Fluorosilicone Fluid — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -200

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -200 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -200 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -220

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 1

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -220 | 1 | 1 | 1 | X | X | X | X | X | 1 | X | X | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -220 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -3

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -3 | 2 | 1 | 1 | 1 | 2 | 1 | 1 | 1 | 1 | 1 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -3 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -33

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -33 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -33 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -4

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -4 | 2 | 1 | 1 | 1 | 2 | 1 | 1 | 1 | 1 | 1 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -4 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -44

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -44 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -44 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -5

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -5 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -5 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -510

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -510 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -510 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -55

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -55 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -55 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -550

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -550 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -550 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -704

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -704 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -704 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -705

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -705 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -705 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning -710

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 3

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning -710 | 2 | 1 | 1 | 1 | 3 | 1 | 1 | 1 | 1 | 1 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning -710 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Corning F-61

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 1

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Corning F-61 | 1 | 1 | 1 | X | X | X | X | X | 1 | X | X | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-2>

Dow Corning F-61 — Chemical resistance ratings for common elastomers


**Chemical:** Dow Guard

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 1

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 3

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dow Guard | 1 | 1 | 1 | 1 | 1 | 1 | 3 | 1 | 1 | 3 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Dow Guard — Chemical resistance ratings for common elastomers


**Chemical:** Dowanol P Mix

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dowanol P Mix | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Dowanol P Mix — Chemical resistance ratings for common elastomers


**Chemical:** Dowtherm, 209

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 2

**SBR:** X

**Silicone (VMQ):** 3

**Butyl (IIR):** 2

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 4

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dowtherm, 209 | 3 | 1 | 2 | X | 3 | 2 | X | X | 4 | X | 3 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Dowtherm, 209 — Chemical resistance ratings for common elastomers


**Chemical:** Dowtherm, A

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dowtherm, A | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Dowtherm, A — Chemical resistance ratings for common elastomers


**Chemical:** Dowtherm, E

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dowtherm, E | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Dowtherm, E — Chemical resistance ratings for common elastomers


**Chemical:** Drinking Water

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 2

**SBR:** 1

**Silicone (VMQ):** 1

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Drinking Water | 1 | 1 | 2 | 1 | 1 | 1 | 4 | 1 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Drinking Water — Chemical resistance ratings for common elastomers


**Chemical:** Dry Cleaning Fluids

**Nitrile (NBR):** 3

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Dry Cleaning Fluids | 3 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Dry Cleaning Fluids — Chemical resistance ratings for common elastomers


**Chemical:** DTE 20 Series, Mobil

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 1

**SBR:** X

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 2

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> DTE 20 Series, Mobil | 2 | 4 | 1 | X | 4 | 4 | 2 | 2 | 1 | 1 | 2 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

DTE 20 Series, Mobil — Chemical resistance ratings for common elastomers


**Chemical:** DTE named series, Mobil, light-heavy

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 3

**Butyl (IIR):** 4

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** 2

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> DTE named series, Mobil, light-heavy | 1 | 4 | 2 | 4 | 3 | 4 | X | 1 | 1 | 1 | 1 | 2 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

DTE named series, Mobil, light-heavy — Chemical resistance ratings for common elastomers


**Chemical:** Elco 28-EP lubricant

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 3

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Elco 28-EP lubricant | 1 | 4 | 3 | 4 | 2 | 4 | 1 | 4 | 1 | 1 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Elco 28-EP lubricant — Chemical resistance ratings for common elastomers


**Chemical:** Epichlorohydrin

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Epichlorohydrin | 4 | 2 | 4 | 4 | 4 | 2 | 4 | 4 | 4 | 4 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Epichlorohydrin — Chemical resistance ratings for common elastomers


**Chemical:** Epoxy Resins

**Nitrile (NBR):** X

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** 1

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 4

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Epoxy Resins | X | 1 | 1 | X | X | 1 | X | X | 4 | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Epoxy Resins — Chemical resistance ratings for common elastomers


**Chemical:** Erucic Acid

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Erucic Acid | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Erucic Acid — Chemical resistance ratings for common elastomers


**Chemical:** Esam-6 Fluid

**Nitrile (NBR):** X

**EPDM:** 1

**Neoprene (CR):** 2

**SBR:** 1

**Silicone (VMQ):** X

**Butyl (IIR):** 2

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 2

**Viton (FKM):** 4

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esam-6 Fluid | X | 1 | 2 | 1 | X | 2 | X | 2 | 4 | X | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esam-6 Fluid — Chemical resistance ratings for common elastomers


**Chemical:** Esso Fuel 208

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 3

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esso Fuel 208 | 1 | 4 | 2 | 4 | 4 | 4 | 1 | 3 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esso Fuel 208 — Chemical resistance ratings for common elastomers


**Chemical:** Esso Golden Gasoline

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esso Golden Gasoline | 2 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esso Golden Gasoline — Chemical resistance ratings for common elastomers


**Chemical:** Esso Motor Oil

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 3

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esso Motor Oil | 1 | 4 | 3 | 4 | 4 | 4 | 1 | 4 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esso Motor Oil — Chemical resistance ratings for common elastomers


**Chemical:** Esso Transmission Fluid (Type A)

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esso Transmission Fluid (Type A) | 1 | 4 | 2 | 4 | 4 | 4 | 1 | 4 | 1 | 3 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esso Transmission Fluid (Type A) — Chemical resistance ratings for common elastomers


**Chemical:** Esso WS2812 (MIL-L-7808A)

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 2

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esso WS2812 (MIL-L-7808A) | 1 | 4 | 4 | 4 | 4 | 4 | 2 | 4 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esso WS2812 (MIL-L-7808A) — Chemical resistance ratings for common elastomers


**Chemical:** Esso XP90-EP Lubricant

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 1

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esso XP90-EP Lubricant | 1 | 4 | 2 | 4 | 4 | 4 | 1 | 2 | 1 | 1 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esso XP90-EP Lubricant — Chemical resistance ratings for common elastomers


**Chemical:** Esstic 42, 43

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Esstic 42, 43 | 1 | 4 | 2 | 4 | 4 | 4 | 1 | 4 | 1 | 2 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Esstic 42, 43 — Chemical resistance ratings for common elastomers


**Chemical:** Ethane

**Nitrile (NBR):** 1

**EPDM:** 4

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 1

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethane | 1 | 4 | 2 | 4 | 4 | 4 | 1 | 2 | 1 | 3 | 3 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethane — Chemical resistance ratings for common elastomers


**Chemical:** Ethanol Amine

**Nitrile (NBR):** 2

**EPDM:** 1

**Neoprene (CR):** 2

**SBR:** 2

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 3

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethanol Amine | 2 | 1 | 2 | 2 | 2 | 2 | 4 | 3 | 4 | 3 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethanol Amine — Chemical resistance ratings for common elastomers


**Chemical:** Ethanol

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethanol | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethanol — Chemical resistance ratings for common elastomers


**Chemical:** Ethers

**Nitrile (NBR):** 4

**EPDM:** 3

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 3

**Hypalon (CSM):** 4

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethers | 4 | 3 | 4 | 4 | 4 | 4 | 3 | 4 | 3 | 2 | 3 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethers — Chemical resistance ratings for common elastomers


**Chemical:** Ethoxyethyl Acetate (EGMEEA)

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethoxyethyl Acetate (EGMEEA) | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethoxyethyl Acetate (EGMEEA) — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Acetate-Organic Ester

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Acetate-Organic Ester | 4 | 2 | 4 | 4 | 2 | 2 | 4 | 4 | 4 | 4 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Acetate-Organic Ester — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Acetoacetate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 3

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Acetoacetate | 4 | 2 | 4 | 3 | 2 | 2 | 4 | 4 | 4 | 4 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Acetoacetate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Acrylate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Acrylate | 4 | 2 | 4 | 4 | 2 | 2 | 4 | 4 | 4 | 4 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Acrylate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Alcohol

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Alcohol | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Alcohol — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Ammonium Dichloride

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Ammonium Dichloride | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Ammonium Dichloride — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Benzene

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Benzene | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Benzene — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Benzoate

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Benzoate | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Benzoate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Bromide

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Bromide | 2 | 4 | 4 | X | X | 4 | X | 4 | 1 | X | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Bromide — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Cellosolve

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Cellosolve | 4 | 2 | 4 | 4 | 4 | 2 | 4 | 4 | 4 | 4 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Cellosolve — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Cellulose

**Nitrile (NBR):** 2

**EPDM:** 2

**Neoprene (CR):** 2

**SBR:** 2

**Silicone (VMQ):** 2

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 2

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Cellulose | 2 | 2 | 2 | 2 | 2 | 2 | 4 | 2 | 4 | 2 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Cellulose — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Chloride

**Nitrile (NBR):** 1

**EPDM:** 3

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 3

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Chloride | 1 | 3 | 4 | 4 | 4 | 4 | 3 | 4 | 1 | 2 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Chloride — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Chlorocarbonate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Chlorocarbonate | 4 | 2 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Chlorocarbonate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Chloroformate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 3

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Chloroformate | 4 | 2 | 4 | 4 | 4 | 3 | 4 | 4 | 4 | 4 | 4 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Chloroformate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Ether

**Nitrile (NBR):** 3

**EPDM:** 3

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 3

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 4

**Polyurethane (AU/EU):** 2

**Fluorosilicone (FVMQ):** 3

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Ether | 3 | 3 | 4 | 4 | 4 | 3 | 4 | 4 | 4 | 2 | 3 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Ether — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Formate

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 2

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Formate | 4 | 2 | 2 | 4 | X | 2 | X | 2 | 1 | X | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Formate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Hexanol

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Hexanol | 1 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 1 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Hexanol — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Lactate

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Lactate | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Lactate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Mercaptan

**Nitrile (NBR):** 4

**EPDM:** X

**Neoprene (CR):** 3

**SBR:** 4

**Silicone (VMQ):** 3

**Butyl (IIR):** 4

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 3

**Viton (FKM):** 2

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Mercaptan | 4 | X | 3 | 4 | 3 | 4 | X | 3 | 2 | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Mercaptan — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Nitrite

**Nitrile (NBR):** 3

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 1

**Silicone (VMQ):** 2

**Butyl (IIR):** 1

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 1

**Viton (FKM):** 3

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Nitrite | 3 | 1 | 1 | 1 | 2 | 1 | 4 | 1 | 3 | 4 | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Nitrite — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Oxalate

**Nitrile (NBR):** 4

**EPDM:** 1

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 2

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Oxalate | 4 | 1 | 4 | 4 | 4 | 4 | 4 | 4 | 2 | X | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Oxalate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Pentachlorobenzene

**Nitrile (NBR):** 4

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Pentachlorobenzene | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 4 | 1 | 4 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Pentachlorobenzene — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Pyridine

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Pyridine | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Pyridine — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Silicate

**Nitrile (NBR):** 1

**EPDM:** 1

**Neoprene (CR):** 1

**SBR:** 2

**Silicone (VMQ):** X

**Butyl (IIR):** 1

**Polyacrylate (ACM):** X

**Hypalon (CSM):** 2

**Viton (FKM):** 1

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** 1

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Silicate | 1 | 1 | 1 | 2 | X | 1 | X | 2 | 1 | X | 1 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Silicate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Stearate

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Stearate | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Stearate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Sulfate

**Nitrile (NBR):** X

**EPDM:** 1

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** 4

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** 1

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Sulfate | X | 1 | X | X | X | X | X | X | 4 | X | X | 1 | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Sulfate — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Tertiary Butyl Ether

**Nitrile (NBR):** X

**EPDM:** X

**Neoprene (CR):** X

**SBR:** X

**Silicone (VMQ):** X

**Butyl (IIR):** X

**Polyacrylate (ACM):** X

**Hypalon (CSM):** X

**Viton (FKM):** X

**Polyurethane (AU/EU):** X

**Fluorosilicone (FVMQ):** X

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Tertiary Butyl Ether | X | X | X | X | X | X | X | X | X | X | X | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Tertiary Butyl Ether — Chemical resistance ratings for common elastomers


**Chemical:** Ethyl Valerate

**Nitrile (NBR):** 2

**EPDM:** 4

**Neoprene (CR):** 4

**SBR:** 4

**Silicone (VMQ):** X

**Butyl (IIR):** 4

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** 1

**Polyurethane (AU/EU):** 3

**Fluorosilicone (FVMQ):** 2

**Aflas (TFE/P):** X

**Kalrez (FFKM):** 1

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethyl Valerate | 2 | 4 | 4 | 4 | X | 4 | 4 | 4 | 1 | 3 | 2 | X | 1 |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethyl Valerate — Chemical resistance ratings for common elastomers


**Chemical:** Ethylacrylic Acid

**Nitrile (NBR):** 4

**EPDM:** 2

**Neoprene (CR):** 2

**SBR:** 4

**Silicone (VMQ):** 4

**Butyl (IIR):** 2

**Polyacrylate (ACM):** 4

**Hypalon (CSM):** 4

**Viton (FKM):** X

**Polyurethane (AU/EU):** 4

**Fluorosilicone (FVMQ):** 4

**Aflas (TFE/P):** X

**Kalrez (FFKM):** X

**Rating scale:** 1 = Satisfactory, 2 = Fair, 3 = Doubtful, 4 = Unsatisfactory, X = Insufficient Data

> Ethylacrylic Acid | 4 | 2 | 2 | 4 | 4 | 2 | 4 | 4 | X | 4 | 4 | X | X |

Source: <https://mykin.com/rubber-chemical-resistance-chart-3>

Ethylacrylic Acid — Chemical resistance ratings for common elastomers